#------------------------------------------------------------------------------
#$Date: 2023-04-26 01:58:07 +0300 (Wed, 26 Apr 2023) $
#$Revision: 282838 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/71/28/7712870.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7712870
loop_
_publ_author_name
'Ablott, Timothy'
'Lu, Kim'
'Wei, Tao'
'Zhang, Yingjie'
_publ_section_title
;
 Exploring the influence of pH on the structural intricacies of uranium
 oxide hydrates containing both Cd(II) and K(I) ions
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D3DT00630A
_journal_year                    2023
_chemical_formula_moiety         'Cd0.5 K2.5 O39 U11'
_chemical_formula_sum            'Cd0.5 K2.5 O39 U11'
_chemical_formula_weight         3396.28
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_primary     dual
_audit_creation_date             2022-12-16
_audit_creation_method
;
Olex2 1.5
(compiled 2021.12.09 svn.r5202d8cf for OlexSys, GUI svn.r6439)
;
_audit_update_record
;
2023-02-25 deposited with the CCDC.	2023-04-25 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 104.23(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.589(2)
_cell_length_b                   21.125(4)
_cell_length_c                   14.596(3)
_cell_measurement_reflns_used    16000
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      24.996
_cell_measurement_theta_min      1.928
_cell_volume                     3463.7(12)
_computing_data_collection       'BlueIce (McPhillips, et al., 2002)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.981
_diffrn_measurement_device_type  'Eiger Detector'
_diffrn_measurement_method       'π  scans'
_diffrn_radiation_type
'silicon double crystal monochromated synchrotron'
_diffrn_radiation_wavelength     0.71086
_diffrn_reflns_av_R_equivalents  0.1056
_diffrn_reflns_av_unetI/netI     0.0643
_diffrn_reflns_Laue_measured_fraction_full 0.981
_diffrn_reflns_Laue_measured_fraction_max 0.981
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            19668
_diffrn_reflns_point_group_measured_fraction_full 0.981
_diffrn_reflns_point_group_measured_fraction_max 0.981
_diffrn_reflns_theta_full        24.996
_diffrn_reflns_theta_max         24.996
_diffrn_reflns_theta_min         1.928
_diffrn_source                   'Australian Synchrotron MX2'
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    51.941
_exptl_absorpt_correction_T_max  0.4344
_exptl_absorpt_correction_T_min  0.3701
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.2137 before and 0.0857 after correction.
The Ratio of minimum to maximum transmission is 0.8520.
The λ/2 correction factor is 0.0015.
;
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    6.513
_exptl_crystal_description       needle
_exptl_crystal_F_000             5582
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.010
_exptl_crystal_size_min          0.004
_refine_diff_density_max         11.137
_refine_diff_density_min         -2.932
_refine_diff_density_rms         0.895
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.114
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     204
_refine_ls_number_reflns         3001
_refine_ls_number_restraints     347
_refine_ls_restrained_S_all      1.053
_refine_ls_R_factor_all          0.0634
_refine_ls_R_factor_gt           0.0538
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0641P)²+242.9001P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1327
_refine_ls_wR_factor_ref         0.1488
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2426
_reflns_number_total             3001
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3dt00630a2.cif
_cod_data_source_block           c2byc_a
_cod_original_cell_volume        3463.8(13)
_cod_original_sg_symbol_H-M      C2/c
_cod_original_formula_sum        'Cd0.50 K2.50 O39 U11'
_cod_database_code               7712870
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(O2) = Uanis(O3) = Uanis(O4) = Uanis(O7) = Uanis(O8) = Uanis(O10) =
Uanis(O12) = Uanis(O14) = Uanis(O15)
2. Rigid body (RIGU) restrains
 All non-hydrogen atoms
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
3. Others
 Fixed Sof: Cd1(0.25) K2(0.375) K3(0.375) O6(0.5)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.750000 0.750000 0.500000 0.0170(3) Uani 1 2 d S . P . .
U2 U 0.44583(7) 0.75079(3) 0.50410(5) 0.0125(2) Uani 1 1 d . . . . .
U3 U 0.25394(6) 0.58899(3) 0.51802(5) 0.0093(2) Uani 1 1 d . . . . .
U4 U -0.06004(7) 0.57993(3) 0.51772(5) 0.0076(2) Uani 1 1 d . . . . .
U5 U -0.17937(7) 0.57483(3) 0.72669(6) 0.0120(2) Uani 1 1 d . . . . .
U6 U -0.42786(7) 0.57984(3) 0.52290(5) 0.0081(2) Uani 1 1 d . . . . .
Cd1 Cd 1.000000 0.82046(19) 0.750000 0.0133(8) Uani 0.5 2 d S T P . .
K1 K 0.000000 0.6161(4) 0.250000 0.0280(16) Uani 1 2 d S T P . .
K2 K -0.500000 0.4889(4) 0.750000 0.0164(17) Uani 0.75 2 d S T P . .
K3 K 0.500000 0.6641(5) 0.750000 0.039(3) Uani 0.75 2 d S T P . .
O1 O 0.8268(16) 0.7776(8) 0.6533(13) 0.037(4) Uani 1 1 d . . . . .
O2 O 0.6313(13) 0.6909(6) 0.5334(10) 0.0185(11) Uani 1 1 d . . . . .
O3 O 0.6172(13) 0.8113(6) 0.4842(10) 0.0185(11) Uani 1 1 d . . . . .
O4 O 0.4803(13) 0.7701(6) 0.6260(10) 0.0185(11) Uani 1 1 d . . . . .
O5 O 0.4138(15) 0.7284(7) 0.3810(11) 0.029(3) Uani 1 1 d . . . . .
O6 O 0.258(3) 0.7538(15) 0.5319(19) 0.023(6) Uani 0.5 1 d . . P . .
O7 O 0.4179(13) 0.6465(6) 0.5450(11) 0.0185(11) Uani 1 1 d . . . . .
O8 O 0.2830(14) 0.5710(6) 0.6515(11) 0.0185(11) Uani 1 1 d . . . . .
O9 O 0.2244(13) 0.6113(8) 0.3945(10) 0.023(3) Uani 1 1 d . . . . .
O10 O 0.1006(13) 0.5243(6) 0.4936(11) 0.0185(11) Uani 1 1 d . . . . .
O11 O 0.1008(13) 0.6451(7) 0.5323(11) 0.019(3) Uani 1 1 d . . . . .
O12 O -0.0062(14) 0.5745(6) 0.6551(11) 0.0185(11) Uani 1 1 d . . . . .
O13 O -0.1203(14) 0.5861(6) 0.3896(11) 0.015(3) Uani 1 1 d . . . . .
O14 O -0.2288(14) 0.5786(6) 0.5629(11) 0.0185(11) Uani 1 1 d . . . . .
O15 O -0.1683(13) 0.4908(7) 0.7256(11) 0.0185(11) Uani 1 1 d . . . . .
O16 O -0.1838(12) 0.6588(6) 0.7314(10) 0.015(3) Uani 1 1 d . . . . .
O17 O -0.4530(13) 0.5937(6) 0.3980(10) 0.015(3) Uani 1 1 d . . . . .
O18 O -0.3925(12) 0.5692(6) 0.6549(11) 0.016(3) Uani 1 1 d . . . . .
O19 O -0.3973(12) 0.4764(6) 0.4941(10) 0.015(3) Uani 1 1 d . . . . .
O20 O 1.1563(13) 0.8932(8) 0.7503(10) 0.025(4) Uani 1 1 d . . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
U2 U1 U2 180.0 7_666 . ?
O1 U1 U2 82.4(5) 7_666 . ?
O1 U1 U2 97.6(5) 7_666 7_666 ?
O1 U1 U2 97.6(5) . . ?
O1 U1 U2 82.4(5) . 7_666 ?
O1 U1 O1 180.0 7_666 . ?
O2 U1 U2 41.7(4) . . ?
O2 U1 U2 41.7(4) 7_666 7_666 ?
O2 U1 U2 138.3(4) . 7_666 ?
O2 U1 U2 138.3(4) 7_666 . ?
O2 U1 O1 87.3(6) 7_666 . ?
O2 U1 O1 92.7(6) 7_666 7_666 ?
O2 U1 O1 87.3(6) . 7_666 ?
O2 U1 O1 92.7(6) . . ?
O2 U1 O2 180.0 . 7_666 ?
O3 U1 U2 41.5(4) 7_666 7_666 ?
O3 U1 U2 138.5(4) 7_666 . ?
O3 U1 U2 41.5(4) . . ?
O3 U1 U2 138.5(4) . 7_666 ?
O3 U1 O1 87.0(6) 7_666 . ?
O3 U1 O1 93.0(6) 7_666 7_666 ?
O3 U1 O1 87.0(6) . 7_666 ?
O3 U1 O1 93.0(6) . . ?
O3 U1 O2 82.9(6) . . ?
O3 U1 O2 97.1(6) 7_666 . ?
O3 U1 O2 82.9(6) 7_666 7_666 ?
O3 U1 O2 97.1(6) . 7_666 ?
O3 U1 O3 180.0(8) 7_666 . ?
U1 U2 U4 68.858(19) . 7_566 ?
U1 U2 U6 68.716(19) . 1_655 ?
U1 U2 K3 94.41(3) . . ?
U4 U2 U6 137.57(3) 7_566 1_655 ?
U4 U2 K3 121.72(13) 7_566 . ?
U6 U2 K3 61.97(13) 1_655 . ?
O2 U2 U1 33.1(3) . . ?
O2 U2 U4 101.0(3) . 7_566 ?
O2 U2 U6 37.3(3) . 1_655 ?
O2 U2 K3 70.3(3) . . ?
O3 U2 U1 32.6(3) . . ?
O3 U2 U4 36.6(3) . 7_566 ?
O3 U2 U6 101.1(3) . 1_655 ?
O3 U2 K3 113.6(4) . . ?
O3 U2 O2 65.5(5) . . ?
O4 U2 U1 92.2(5) . . ?
O4 U2 U4 82.7(5) . 7_566 ?
O4 U2 U6 98.9(4) . 1_655 ?
O4 U2 K3 41.1(5) . . ?
O4 U2 O2 88.4(6) . . ?
O4 U2 O3 90.6(6) . . ?
O4 U2 O5 177.9(7) . . ?
O4 U2 O6 101.8(9) . 7_566 ?
O4 U2 O6 78.8(8) . . ?
O4 U2 O7 88.3(6) . . ?
O4 U2 O11 89.7(6) . 7_566 ?
O5 U2 U1 86.8(6) . . ?
O5 U2 U4 98.7(5) . 7_566 ?
O5 U2 U6 79.0(5) . 1_655 ?
O5 U2 K3 137.1(5) . . ?
O5 U2 O2 89.8(6) . . ?
O5 U2 O3 89.6(6) . . ?
O5 U2 O6 79.2(9) . 7_566 ?
O5 U2 O6 102.1(9) . . ?
O5 U2 O7 90.0(6) . . ?
O5 U2 O11 92.4(6) . 7_566 ?
O6 U2 U1 165.9(7) 7_566 . ?
O6 U2 U1 171.0(7) . . ?
O6 U2 U4 110.3(8) . 7_566 ?
O6 U2 U4 112.1(8) 7_566 7_566 ?
O6 U2 U6 109.0(8) 7_566 1_655 ?
O6 U2 U6 111.6(8) . 1_655 ?
O6 U2 K3 78.4(7) . . ?
O6 U2 K3 96.5(7) 7_566 . ?
O6 U2 O2 144.2(9) . . ?
O6 U2 O2 146.3(9) 7_566 . ?
O6 U2 O3 144.9(9) 7_566 . ?
O6 U2 O3 146.7(8) . . ?
O6 U2 O6 23.0(13) 7_566 . ?
O6 U2 O7 77.6(9) . . ?
O6 U2 O7 79.5(9) 7_566 . ?
O6 U2 O11 79.5(9) 7_566 7_566 ?
O7 U2 U1 101.6(4) . . ?
O7 U2 U4 166.5(4) . 7_566 ?
O7 U2 U6 34.3(4) . 1_655 ?
O7 U2 K3 47.7(4) . . ?
O7 U2 O2 68.6(5) . . ?
O7 U2 O3 134.1(5) . . ?
O11 U2 U1 100.3(3) 7_566 . ?
O11 U2 U4 32.6(4) 7_566 7_566 ?
O11 U2 U6 166.2(3) 7_566 1_655 ?
O11 U2 K3 129.2(4) 7_566 . ?
O11 U2 O2 133.2(5) 7_566 . ?
O11 U2 O3 67.8(5) 7_566 . ?
O11 U2 O6 80.6(9) 7_566 . ?
O11 U2 O7 158.0(5) 7_566 . ?
U2 U3 K1 64.52(9) 7_566 . ?
U2 U3 K3 90.58(13) 7_566 . ?
U4 U3 U2 59.658(19) . 7_566 ?
U4 U3 U5 63.70(3) . 2_556 ?
U4 U3 U6 173.89(3) . 1_655 ?
U4 U3 K1 63.10(3) . . ?
U4 U3 K3 120.32(4) . . ?
U5 U3 U2 83.58(3) 2_556 7_566 ?
U5 U3 K1 126.39(2) 2_556 . ?
U5 U3 K3 62.44(5) 2_556 . ?
U6 U3 U2 126.43(3) 1_655 7_566 ?
U6 U3 U5 114.80(4) 1_655 2_556 ?
U6 U3 K1 118.80(3) 1_655 . ?
U6 U3 K3 61.41(5) 1_655 . ?
K3 U3 K1 149.75(17) . . ?
O7 U3 U2 90.3(3) . 7_566 ?
O7 U3 U4 147.7(4) . . ?
O7 U3 U5 104.2(4) . 2_556 ?
O7 U3 U6 37.8(4) . 1_655 ?
O7 U3 K1 117.0(4) . . ?
O7 U3 K3 42.1(4) . . ?
O8 U3 U2 101.5(4) . 7_566 ?
O8 U3 U4 85.2(5) . . ?
O8 U3 U5 22.8(4) . 2_556 ?
O8 U3 U6 92.6(5) . 1_655 ?
O8 U3 K1 148.3(5) . . ?
O8 U3 K3 48.8(4) . . ?
O8 U3 O7 90.0(6) . . ?
O8 U3 O10 88.5(6) . . ?
O8 U3 O11 87.4(6) . . ?
O8 U3 O19 90.6(6) . 5_566 ?
O9 U3 U2 74.9(5) . 7_566 ?
O9 U3 U4 93.9(5) . . ?
O9 U3 U5 155.0(5) . 2_556 ?
O9 U3 U6 88.6(5) . 1_655 ?
O9 U3 K1 31.1(5) . . ?
O9 U3 K3 129.3(5) . . ?
O9 U3 O7 88.8(6) . . ?
O9 U3 O8 176.2(7) . . ?
O9 U3 O10 93.0(6) . . ?
O9 U3 O11 89.7(6) . . ?
O9 U3 O19 92.6(6) . 5_566 ?
O10 U3 U2 94.7(4) . 7_566 ?
O10 U3 U4 36.9(4) . . ?
O10 U3 U5 75.9(4) . 2_556 ?
O10 U3 U6 137.5(4) . 1_655 ?
O10 U3 K1 65.9(4) . . ?
O10 U3 K3 137.1(4) . . ?
O10 U3 O7 175.0(5) . . ?
O11 U3 U2 25.5(4) . 7_566 ?
O11 U3 U4 36.3(4) . . ?
O11 U3 U5 65.8(4) . 2_556 ?
O11 U3 U6 149.4(4) . 1_655 ?
O11 U3 K1 68.0(4) . . ?
O11 U3 K3 97.2(4) . . ?
O11 U3 O7 111.6(5) . . ?
O11 U3 O10 73.1(5) . . ?
O11 U3 O19 173.9(5) . 5_566 ?
O19 U3 U2 160.3(3) 5_566 7_566 ?
O19 U3 U4 137.8(3) 5_566 . ?
O19 U3 U5 111.4(4) 5_566 2_556 ?
O19 U3 U6 36.4(3) 5_566 1_655 ?
O19 U3 K1 111.7(4) 5_566 . ?
O19 U3 K3 85.7(4) 5_566 . ?
O19 U3 O7 74.1(5) 5_566 . ?
O19 U3 O10 101.1(5) 5_566 . ?
U2 U4 U5 85.97(2) 7_566 2_556 ?
U3 U4 U2 65.67(2) . 7_566 ?
U3 U4 U4 69.01(3) . 5_566 ?
U3 U4 U5 125.77(4) . . ?
U3 U4 U5 62.89(3) . 2_556 ?
U4 U4 U2 132.85(4) 5_566 7_566 ?
U4 U4 U5 84.82(3) 5_566 2_556 ?
U5 U4 U2 107.76(2) . 7_566 ?
U5 U4 U4 108.65(3) . 5_566 ?
U5 U4 U5 62.97(3) . 2_556 ?
O3 U4 U2 37.5(3) 7_566 7_566 ?
O3 U4 U3 102.9(4) 7_566 . ?
O3 U4 U4 168.2(4) 7_566 5_566 ?
O3 U4 U5 99.3(4) 7_566 2_556 ?
O3 U4 U5 82.9(4) 7_566 . ?
O10 U4 U2 98.9(3) . 7_566 ?
O10 U4 U2 166.5(4) 5_566 7_566 ?
O10 U4 U3 35.1(3) . . ?
O10 U4 U3 104.0(4) 5_566 . ?
O10 U4 U4 34.3(3) . 5_566 ?
O10 U4 U4 35.2(4) 5_566 5_566 ?
O10 U4 U5 126.9(4) . . ?
O10 U4 U5 85.2(4) 5_566 . ?
O10 U4 U5 74.4(4) . 2_556 ?
O10 U4 U5 97.1(4) 5_566 2_556 ?
O10 U4 O3 152.6(5) 5_566 7_566 ?
O10 U4 O3 136.2(5) . 7_566 ?
O10 U4 O10 69.6(6) 5_566 . ?
O10 U4 O11 138.4(5) 5_566 . ?
O11 U4 U2 32.8(4) . 7_566 ?
O11 U4 U3 34.5(3) . . ?
O11 U4 U4 103.5(3) . 5_566 ?
O11 U4 U5 64.8(4) . 2_556 ?
O11 U4 U5 114.1(4) . . ?
O11 U4 O3 68.9(5) . 7_566 ?
O11 U4 O10 69.5(5) . . ?
O12 U4 U2 96.3(4) . 7_566 ?
O12 U4 U3 86.3(5) . . ?
O12 U4 U4 93.1(4) . 5_566 ?
O12 U4 U5 39.6(5) . . ?
O12 U4 U5 23.4(5) . 2_556 ?
O12 U4 O3 94.9(5) . 7_566 ?
O12 U4 O10 93.5(6) . . ?
O12 U4 O10 91.5(5) . 5_566 ?
O12 U4 O11 83.8(6) . . ?
O12 U4 O14 77.0(6) . . ?
O13 U4 U2 84.4(4) . 7_566 ?
O13 U4 U3 97.3(5) . . ?
O13 U4 U4 89.1(4) . 5_566 ?
O13 U4 U5 136.7(5) . . ?
O13 U4 U5 160.2(5) . 2_556 ?
O13 U4 O3 83.3(5) . 7_566 ?
O13 U4 O10 90.0(6) . . ?
O13 U4 O10 88.6(6) . 5_566 ?
O13 U4 O11 98.6(6) . . ?
O13 U4 O12 176.3(7) . . ?
O13 U4 O14 99.3(6) . . ?
O14 U4 U2 112.5(3) . 7_566 ?
O14 U4 U3 163.0(4) . . ?
O14 U4 U4 114.6(3) . 5_566 ?
O14 U4 U5 37.4(4) . . ?
O14 U4 U5 100.4(4) . 2_556 ?
O14 U4 O3 75.7(5) . 7_566 ?
O14 U4 O10 79.9(5) . 5_566 ?
O14 U4 O10 147.9(5) . . ?
O14 U4 O11 137.8(5) . . ?
U3 U5 U4 53.42(2) 2_556 2_556 ?
U3 U5 U5 106.80(4) 2_556 2_556 ?
U4 U5 U3 168.74(3) . 2_556 ?
U4 U5 U4 116.93(3) . 2_556 ?
U4 U5 U5 63.59(3) . 2_556 ?
U5 U5 U4 53.44(3) 2_556 2_556 ?
U6 U5 U3 116.84(3) . 2_556 ?
U6 U5 U4 169.97(3) . 2_556 ?
U6 U5 U4 72.46(3) . . ?
U6 U5 U5 136.05(4) . 2_556 ?
O8 U5 U3 18.4(4) 2_556 2_556 ?
O8 U5 U4 70.8(4) 2_556 2_556 ?
O8 U5 U4 172.3(4) 2_556 . ?
O8 U5 U5 124.1(4) 2_556 2_556 ?
O8 U5 U6 99.8(4) 2_556 . ?
O8 U5 O12 157.6(5) 2_556 . ?
O8 U5 O12 89.5(5) 2_556 2_556 ?
O8 U5 O18 71.0(5) 2_556 . ?
O12 U5 U3 140.2(4) . 2_556 ?
O12 U5 U3 72.2(4) 2_556 2_556 ?
O12 U5 U4 98.3(4) 2_556 . ?
O12 U5 U4 18.8(4) 2_556 2_556 ?
O12 U5 U4 86.9(4) . 2_556 ?
O12 U5 U4 30.1(4) . . ?
O12 U5 U5 33.5(4) . 2_556 ?
O12 U5 U5 34.7(4) 2_556 2_556 ?
O12 U5 U6 170.6(4) 2_556 . ?
O12 U5 U6 102.6(4) . . ?
O12 U5 O12 68.2(6) 2_556 . ?
O12 U5 O18 160.4(5) 2_556 . ?
O14 U5 U3 153.4(4) . 2_556 ?
O14 U5 U4 35.4(4) . . ?
O14 U5 U4 152.2(4) . 2_556 ?
O14 U5 U5 99.0(4) . 2_556 ?
O14 U5 U6 37.0(4) . . ?
O14 U5 O8 136.8(5) . 2_556 ?
O14 U5 O12 65.6(5) . . ?
O14 U5 O12 133.7(6) . 2_556 ?
O14 U5 O18 65.9(5) . . ?
O15 U5 U3 96.6(5) . 2_556 ?
O15 U5 U4 90.0(5) . 2_556 ?
O15 U5 U4 88.8(5) . . ?
O15 U5 U5 85.9(5) . 2_556 ?
O15 U5 U6 93.8(5) . . ?
O15 U5 O8 91.3(6) . 2_556 ?
O15 U5 O12 87.1(6) . 2_556 ?
O15 U5 O12 85.8(6) . . ?
O15 U5 O14 91.4(6) . . ?
O15 U5 O18 90.9(6) . . ?
O16 U5 U3 82.9(4) . 2_556 ?
O16 U5 U4 91.3(4) . . ?
O16 U5 U4 87.6(5) . 2_556 ?
O16 U5 U5 91.8(4) . 2_556 ?
O16 U5 U6 88.7(5) . . ?
O16 U5 O8 88.9(5) . 2_556 ?
O16 U5 O12 90.2(6) . 2_556 ?
O16 U5 O12 93.0(5) . . ?
O16 U5 O14 90.2(6) . . ?
O16 U5 O15 177.4(7) . . ?
O16 U5 O18 91.7(5) . . ?
O18 U5 U3 88.6(4) . 2_556 ?
O18 U5 U4 101.2(4) . . ?
O18 U5 U4 141.8(4) . 2_556 ?
O18 U5 U5 164.5(4) . 2_556 ?
O18 U5 U6 29.0(4) . . ?
O18 U5 O12 131.2(5) . . ?
U2 U6 K3 59.74(13) 1_455 1_455 ?
U3 U6 U2 65.83(2) 1_455 1_455 ?
U3 U6 U6 69.07(3) 1_455 5_466 ?
U3 U6 K3 65.32(4) 1_455 1_455 ?
U5 U6 U2 107.29(2) . 1_455 ?
U5 U6 U3 127.80(3) . 1_455 ?
U5 U6 U6 110.61(3) . 5_466 ?
U5 U6 K3 67.56(4) . 1_455 ?
U6 U6 U2 132.87(4) 5_466 1_455 ?
U6 U6 K3 111.74(13) 5_466 1_455 ?
O2 U6 U2 37.3(3) 1_455 1_455 ?
O2 U6 U3 102.5(3) 1_455 1_455 ?
O2 U6 U5 79.7(3) 1_455 . ?
O2 U6 U6 169.3(3) 1_455 5_466 ?
O2 U6 K3 68.6(4) 1_455 1_455 ?
O7 U6 U2 33.8(3) 1_455 1_455 ?
O7 U6 U3 35.0(3) 1_455 1_455 ?
O7 U6 U5 112.6(4) 1_455 . ?
O7 U6 U6 104.0(3) 1_455 5_466 ?
O7 U6 K3 46.0(4) 1_455 1_455 ?
O7 U6 O2 68.1(5) 1_455 1_455 ?
O14 U6 U2 112.1(3) . 1_455 ?
O14 U6 U3 166.2(4) . 1_455 ?
O14 U6 U5 38.6(4) . . ?
O14 U6 U6 115.0(3) . 5_466 ?
O14 U6 K3 101.5(4) . 1_455 ?
O14 U6 O2 74.9(5) . 1_455 ?
O14 U6 O7 137.6(5) . 1_455 ?
O14 U6 O19 147.5(5) . 5_466 ?
O14 U6 O19 80.7(5) . . ?
O17 U6 U2 79.2(4) . 1_455 ?
O17 U6 U3 93.4(5) . 1_455 ?
O17 U6 U5 137.8(5) . . ?
O17 U6 U6 90.7(4) . 5_466 ?
O17 U6 K3 138.4(4) . 1_455 ?
O17 U6 O2 83.1(6) . 1_455 ?
O17 U6 O7 95.8(6) . 1_455 ?
O17 U6 O14 99.6(6) . . ?
O17 U6 O18 176.0(6) . . ?
O17 U6 O19 93.2(6) . 5_466 ?
O17 U6 O19 87.9(6) . . ?
O18 U6 U2 99.6(4) . 1_455 ?
O18 U6 U3 89.5(4) . 1_455 ?
O18 U6 U5 38.9(4) . . ?
O18 U6 U6 92.9(4) . 5_466 ?
O18 U6 K3 41.1(4) . 1_455 ?
O18 U6 O2 93.6(5) . 1_455 ?
O18 U6 O7 85.0(6) . 1_455 ?
O18 U6 O14 77.3(6) . . ?
O18 U6 O19 94.0(5) . . ?
O18 U6 O19 90.8(6) . 5_466 ?
O19 U6 U2 163.0(4) . 1_455 ?
O19 U6 U2 99.5(3) 5_466 1_455 ?
O19 U6 U3 104.4(3) . 1_455 ?
O19 U6 U3 34.4(3) 5_466 1_455 ?
O19 U6 U5 125.2(4) 5_466 . ?
O19 U6 U5 89.7(4) . . ?
O19 U6 U6 35.3(3) . 5_466 ?
O19 U6 U6 34.7(3) 5_466 5_466 ?
O19 U6 K3 87.8(3) 5_466 1_455 ?
O19 U6 K3 130.6(4) . 1_455 ?
O19 U6 O2 152.1(5) . 1_455 ?
O19 U6 O2 136.6(5) 5_466 1_455 ?
O19 U6 O7 69.3(5) 5_466 1_455 ?
O19 U6 O7 139.3(5) . 1_455 ?
O19 U6 O19 70.0(5) . 5_466 ?
O1 Cd1 K2 112.8(4) 2_756 3_655 ?
O1 Cd1 K2 112.8(4) . 3_655 ?
O1 Cd1 O1 134.3(8) . 2_756 ?
O1 Cd1 O5 82.0(6) . 8_566 ?
O1 Cd1 O5 80.1(6) . 7_666 ?
O1 Cd1 O5 80.1(6) 2_756 8_566 ?
O1 Cd1 O5 82.0(6) 2_756 7_666 ?
O1 Cd1 O20 142.6(6) . . ?
O1 Cd1 O20 73.0(6) . 2_756 ?
O1 Cd1 O20 73.0(6) 2_756 . ?
O1 Cd1 O20 142.6(6) 2_756 2_756 ?
O5 Cd1 K2 113.6(3) 8_566 3_655 ?
O5 Cd1 K2 113.6(3) 7_666 3_655 ?
O5 Cd1 O5 132.8(7) 7_666 8_566 ?
O20 Cd1 K2 49.7(4) 2_756 3_655 ?
O20 Cd1 K2 49.7(4) . 3_655 ?
O20 Cd1 O5 133.8(5) 2_756 7_666 ?
O20 Cd1 O5 80.0(5) . 7_666 ?
O20 Cd1 O5 133.8(5) . 8_566 ?
O20 Cd1 O5 80.0(5) 2_756 8_566 ?
O20 Cd1 O20 99.4(8) . 2_756 ?
U3 K1 U3 164.8(2) 2 . ?
U4 K1 U3 50.60(2) 2 2 ?
U4 K1 U3 125.91(7) . 2 ?
U4 K1 U3 50.60(2) . . ?
U4 K1 U3 125.91(7) 2 . ?
U4 K1 U4 159.1(2) . 2 ?
O4 K1 U3 67.9(3) 7_566 . ?
O4 K1 U3 126.1(3) 7_566 2 ?
O4 K1 U3 126.1(3) 8_465 . ?
O4 K1 U3 67.9(3) 8_465 2 ?
O4 K1 U4 65.7(3) 7_566 . ?
O4 K1 U4 134.8(3) 8_465 . ?
O4 K1 U4 134.8(3) 7_566 2 ?
O4 K1 U4 65.7(3) 8_465 2 ?
O4 K1 O4 72.6(6) 7_566 8_465 ?
O9 K1 U3 18.7(3) 2 2 ?
O9 K1 U3 159.7(3) . 2 ?
O9 K1 U3 159.7(3) 2 . ?
O9 K1 U3 18.7(3) . . ?
O9 K1 U4 69.1(3) 2 2 ?
O9 K1 U4 110.1(3) . 2 ?
O9 K1 U4 69.1(3) . . ?
O9 K1 U4 110.1(3) 2 . ?
O9 K1 O4 112.8(4) . 8_465 ?
O9 K1 O4 70.6(4) . 7_566 ?
O9 K1 O4 112.8(4) 2 7_566 ?
O9 K1 O4 70.6(4) 2 8_465 ?
O9 K1 O9 176.0(7) . 2 ?
O9 K1 O15 56.0(4) . 5_566 ?
O9 K1 O15 56.0(4) 2 6_565 ?
O9 K1 O15 120.4(5) 2 5_566 ?
O9 K1 O15 120.4(5) . 6_565 ?
O13 K1 U3 70.3(3) . . ?
O13 K1 U3 106.1(3) . 2 ?
O13 K1 U3 106.1(3) 2 . ?
O13 K1 U3 70.3(3) 2 2 ?
O13 K1 U4 19.9(3) . . ?
O13 K1 U4 19.9(3) 2 2 ?
O13 K1 U4 149.1(3) . 2 ?
O13 K1 U4 149.1(3) 2 . ?
O13 K1 O4 130.0(4) . 8_465 ?
O13 K1 O4 73.7(4) 2 8_465 ?
O13 K1 O4 130.0(4) 2 7_566 ?
O13 K1 O4 73.7(4) . 7_566 ?
O13 K1 O9 88.9(4) . . ?
O13 K1 O9 90.2(4) 2 . ?
O13 K1 O9 88.9(4) 2 2 ?
O13 K1 O9 90.2(4) . 2 ?
O13 K1 O13 154.0(6) . 2 ?
O13 K1 O15 58.9(4) 2 5_566 ?
O13 K1 O15 58.9(4) . 6_565 ?
O13 K1 O15 99.9(4) 2 6_565 ?
O13 K1 O15 99.9(4) . 5_566 ?
O15 K1 U3 106.9(3) 6_565 . ?
O15 K1 U3 60.4(3) 6_565 2 ?
O15 K1 U3 106.9(3) 5_566 2 ?
O15 K1 U3 60.4(3) 5_566 . ?
O15 K1 U4 90.3(3) 5_566 . ?
O15 K1 U4 73.6(3) 5_566 2 ?
O15 K1 U4 90.3(3) 6_565 2 ?
O15 K1 U4 73.6(3) 6_565 . ?
O15 K1 O4 129.8(4) 6_565 7_566 ?
O15 K1 O4 126.5(4) 5_566 7_566 ?
O15 K1 O4 129.8(4) 5_566 8_465 ?
O15 K1 O4 126.5(4) 6_565 8_465 ?
O15 K1 O15 80.0(6) 6_565 5_566 ?
U6 K2 U6 124.0(2) 2_456 . ?
Cd1 K2 U6 118.02(10) 3_345 . ?
Cd1 K2 U6 118.02(10) 3_345 2_456 ?
Cd1 K2 K3 180.0 3_345 1_455 ?
K3 K2 U6 61.98(10) 1_455 . ?
K3 K2 U6 61.98(10) 1_455 2_456 ?
O8 K2 U6 70.5(3) 2_556 2_456 ?
O8 K2 U6 79.0(3) 1_455 2_456 ?
O8 K2 U6 70.5(3) 1_455 . ?
O8 K2 U6 79.0(3) 2_556 . ?
O8 K2 Cd1 124.0(3) 2_556 3_345 ?
O8 K2 Cd1 124.0(3) 1_455 3_345 ?
O8 K2 K3 56.0(3) 1_455 1_455 ?
O8 K2 K3 56.0(3) 2_556 1_455 ?
O8 K2 O8 112.0(6) 2_556 1_455 ?
O17 K2 U6 154.4(3) 6_566 . ?
O17 K2 U6 72.5(3) 6_566 2_456 ?
O17 K2 U6 154.4(3) 5_466 2_456 ?
O17 K2 U6 72.5(3) 5_466 . ?
O17 K2 Cd1 50.2(3) 5_466 3_345 ?
O17 K2 Cd1 50.2(3) 6_566 3_345 ?
O17 K2 K3 129.8(3) 6_566 1_455 ?
O17 K2 K3 129.8(3) 5_466 1_455 ?
O17 K2 O8 90.5(4) 5_466 1_455 ?
O17 K2 O8 90.5(4) 6_566 2_556 ?
O17 K2 O8 135.0(4) 5_466 2_556 ?
O17 K2 O8 135.0(4) 6_566 1_455 ?
O17 K2 O17 100.4(6) 5_466 6_566 ?
O18 K2 U6 21.8(3) . . ?
O18 K2 U6 109.6(4) 2_456 . ?
O18 K2 U6 21.8(3) 2_456 2_456 ?
O18 K2 U6 109.6(4) . 2_456 ?
O18 K2 Cd1 129.2(3) 2_456 3_345 ?
O18 K2 Cd1 129.2(3) . 3_345 ?
O18 K2 K3 50.8(3) . 1_455 ?
O18 K2 K3 50.8(3) 2_456 1_455 ?
O18 K2 O8 80.4(4) . 1_455 ?
O18 K2 O8 80.4(4) 2_456 2_556 ?
O18 K2 O8 57.3(5) . 2_556 ?
O18 K2 O8 57.3(5) 2_456 1_455 ?
O18 K2 O17 141.9(4) . 6_566 ?
O18 K2 O17 91.3(4) . 5_466 ?
O18 K2 O17 141.9(4) 2_456 5_466 ?
O18 K2 O17 91.3(4) 2_456 6_566 ?
O18 K2 O18 101.6(6) . 2_456 ?
O18 K2 O20 149.8(4) . 4_546 ?
O18 K2 O20 94.4(4) 2_456 4_546 ?
O18 K2 O20 94.4(4) . 3_345 ?
O18 K2 O20 149.8(4) 2_456 3_345 ?
O20 K2 U6 94.7(3) 4_546 2_456 ?
O20 K2 U6 128.2(3) 3_345 2_456 ?
O20 K2 U6 128.2(3) 4_546 . ?
O20 K2 U6 94.7(3) 3_345 . ?
O20 K2 Cd1 41.9(4) 4_546 3_345 ?
O20 K2 Cd1 41.9(4) 3_345 3_345 ?
O20 K2 K3 138.1(4) 4_546 1_455 ?
O20 K2 K3 138.1(4) 3_345 1_455 ?
O20 K2 O8 87.2(4) 4_546 1_455 ?
O20 K2 O8 151.9(4) 3_345 1_455 ?
O20 K2 O8 151.9(4) 4_546 2_556 ?
O20 K2 O8 87.2(4) 3_345 2_556 ?
O20 K2 O17 61.2(5) 3_345 6_566 ?
O20 K2 O17 61.2(5) 4_546 5_466 ?
O20 K2 O17 61.8(5) 4_546 6_566 ?
O20 K2 O17 61.8(5) 3_345 5_466 ?
O20 K2 O20 83.7(7) 4_546 3_345 ?
U2 K3 U2 124.6(3) . 2_656 ?
U2 K3 U6 58.295(19) . 1_655 ?
U2 K3 U6 159.47(3) 2_656 1_655 ?
K2 K3 U2 117.71(14) 1_655 2_656 ?
K2 K3 U2 117.71(14) 1_655 . ?
K2 K3 U6 63.78(14) 1_655 1_655 ?
O4 K3 U2 100.5(4) 2_656 . ?
O4 K3 U2 100.5(4) . 2_656 ?
O4 K3 U2 24.1(3) . . ?
O4 K3 U2 24.1(3) 2_656 2_656 ?
O4 K3 U6 79.9(3) . 1_655 ?
O4 K3 U6 150.3(4) 2_656 1_655 ?
O4 K3 K2 141.7(3) . 1_655 ?
O4 K3 K2 141.7(3) 2_656 1_655 ?
O4 K3 O4 76.6(6) 2_656 . ?
O4 K3 O7 59.8(4) 2_656 2_656 ?
O4 K3 O7 134.6(5) 2_656 . ?
O4 K3 O7 59.8(4) . . ?
O4 K3 O7 134.6(5) . 2_656 ?
O4 K3 O8 105.2(4) . . ?
O4 K3 O8 133.7(4) . 2_656 ?
O4 K3 O8 133.7(4) 2_656 . ?
O4 K3 O8 105.2(4) 2_656 2_656 ?
O4 K3 O18 102.5(4) 2_656 2_556 ?
O4 K3 O18 150.8(4) 2_656 1_655 ?
O4 K3 O18 150.8(4) . 2_556 ?
O4 K3 O18 102.5(4) . 1_655 ?
O7 K3 U2 158.1(4) 2_656 . ?
O7 K3 U2 158.1(4) . 2_656 ?
O7 K3 U2 35.9(3) . . ?
O7 K3 U2 35.9(3) 2_656 2_656 ?
O7 K3 U6 35.4(3) . 1_655 ?
O7 K3 U6 134.7(4) 2_656 1_655 ?
O7 K3 K2 82.7(3) 2_656 1_655 ?
O7 K3 K2 82.7(3) . 1_655 ?
O7 K3 O7 165.4(7) 2_656 . ?
O7 K3 O8 56.5(4) . . ?
O7 K3 O8 113.5(4) 2_656 . ?
O7 K3 O8 56.5(4) 2_656 2_656 ?
O7 K3 O8 113.5(4) . 2_656 ?
O8 K3 U2 128.3(3) 2_656 . ?
O8 K3 U2 86.9(3) . . ?
O8 K3 U2 128.3(3) . 2_656 ?
O8 K3 U2 86.9(3) 2_656 2_656 ?
O8 K3 U6 78.5(3) 2_656 1_655 ?
O8 K3 U6 70.2(3) . 1_655 ?
O8 K3 K2 52.6(3) 2_656 1_655 ?
O8 K3 K2 52.6(3) . 1_655 ?
O8 K3 O8 105.2(6) 2_656 . ?
O18 K3 U2 140.3(3) 1_655 2_656 ?
O18 K3 U2 82.9(3) 2_556 2_656 ?
O18 K3 U2 140.3(3) 2_556 . ?
O18 K3 U2 82.9(3) 1_655 . ?
O18 K3 U6 106.9(4) 2_556 1_655 ?
O18 K3 U6 25.4(3) 1_655 1_655 ?
O18 K3 K2 46.1(3) 2_556 1_655 ?
O18 K3 K2 46.1(3) 1_655 1_655 ?
O18 K3 O7 109.4(5) 1_655 2_656 ?
O18 K3 O7 109.4(5) 2_556 . ?
O18 K3 O7 59.5(4) 1_655 . ?
O18 K3 O7 59.5(4) 2_556 2_656 ?
O18 K3 O8 54.0(5) 1_655 2_656 ?
O18 K3 O8 54.0(5) 2_556 . ?
O18 K3 O8 75.2(4) 2_556 2_656 ?
O18 K3 O8 75.2(4) 1_655 . ?
O18 K3 O18 92.1(7) 1_655 2_556 ?
U1 O1 Cd1 140.0(8) . . ?
U1 O2 U2 105.2(6) . . ?
U1 O2 U6 141.5(7) . 1_655 ?
U6 O2 U2 105.4(5) 1_655 . ?
U1 O3 U2 106.0(6) . . ?
U1 O3 U4 146.6(7) . 7_566 ?
U4 O3 U2 105.9(5) 7_566 . ?
U2 O4 K1 139.3(7) . 7_566 ?
U2 O4 K3 114.8(6) . . ?
K3 O4 K1 105.4(5) . 7_566 ?
U2 O5 Cd1 145.0(9) . 7_666 ?
U2 O6 U2 157.0(13) 7_566 . ?
O6 O6 U2 77(4) 7_566 . ?
O6 O6 U2 80(4) 7_566 7_566 ?
U2 O7 U6 111.9(6) . 1_655 ?
U2 O7 K3 96.4(5) . . ?
U3 O7 U2 130.0(6) . . ?
U3 O7 U6 107.2(5) . 1_655 ?
U3 O7 K3 107.5(6) . . ?
U6 O7 K3 98.5(5) 1_655 . ?
U3 O8 U5 138.8(8) . 2_556 ?
U3 O8 K2 119.9(6) . 1_655 ?
U3 O8 K3 104.6(6) . . ?
U5 O8 K2 100.0(5) 2_556 1_655 ?
U5 O8 K3 97.3(5) 2_556 . ?
K2 O8 K3 71.4(4) 1_655 . ?
U3 O9 K1 130.1(7) . . ?
U3 O10 U4 140.0(7) . 5_566 ?
U3 O10 U4 108.0(6) . . ?
U4 O10 U4 110.4(6) 5_566 . ?
U3 O11 U2 130.4(6) . 7_566 ?
U3 O11 U4 109.1(6) . . ?
U4 O11 U2 114.5(6) . 7_566 ?
U4 O12 U5 137.8(8) . 2_556 ?
U4 O12 U5 110.2(7) . . ?
U5 O12 U5 111.8(6) 2_556 . ?
U4 O13 K1 128.6(7) . . ?
U4 O14 U5 107.2(6) . . ?
U4 O14 U6 148.5(8) . . ?
U6 O14 U5 104.3(6) . . ?
U5 O15 K1 144.1(7) . 5_566 ?
U6 O17 K2 130.5(7) . 5_466 ?
U5 O18 K2 111.0(6) . . ?
U5 O18 K3 105.7(5) . 1_455 ?
U6 O18 U5 112.1(7) . . ?
U6 O18 K2 126.3(6) . . ?
U6 O18 K3 113.5(6) . 1_455 ?
K2 O18 K3 83.1(5) . 1_455 ?
U3 O19 U6 109.2(6) 5_566 5_466 ?
U3 O19 U6 140.8(6) 5_566 . ?
U6 O19 U6 110.0(5) . 5_466 ?
Cd1 O20 K2 88.5(5) . 3_655 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 U2 3.5402(10) . ?
U1 U2 3.5402(10) 7_666 ?
U1 O1 2.271(19) 7_666 ?
U1 O1 2.271(19) . ?
U1 O2 2.005(14) . ?
U1 O2 2.005(14) 7_666 ?
U1 O3 1.982(14) . ?
U1 O3 1.982(14) 7_666 ?
U2 U4 3.8535(12) 7_566 ?
U2 U6 3.8811(12) 1_655 ?
U2 K3 3.940(5) . ?
U2 O2 2.439(14) . ?
U2 O3 2.439(15) . ?
U2 O4 1.773(15) . ?
U2 O5 1.805(16) . ?
U2 O6 2.29(3) 7_566 ?
U2 O6 2.31(3) . ?
U2 O7 2.326(14) . ?
U2 O11 2.296(14) 7_566 ?
U3 U4 3.6427(12) . ?
U3 U5 4.0378(13) 2_556 ?
U3 U6 3.6758(12) 1_655 ?
U3 K1 4.3165(19) . ?
U3 K3 4.167(4) . ?
U3 O7 2.208(14) . ?
U3 O8 1.932(16) . ?
U3 O9 1.813(14) . ?
U3 O10 2.200(14) . ?
U3 O11 2.186(14) . ?
U3 O19 2.200(13) 5_566 ?
U4 U4 3.7367(15) 5_566 ?
U4 U5 4.0667(18) 2_556 ?
U4 U5 3.6472(13) . ?
U4 O3 2.389(13) 7_566 ?
U4 O10 2.301(14) . ?
U4 O10 2.249(14) 5_566 ?
U4 O11 2.284(14) . ?
U4 O12 1.951(16) . ?
U4 O13 1.833(15) . ?
U4 O14 2.213(16) . ?
U5 U5 4.0443(17) 2_556 ?
U5 U6 3.5973(17) . ?
U5 O8 2.379(16) 2_556 ?
U5 O12 2.404(16) 2_556 ?
U5 O12 2.480(16) . ?
U5 O14 2.319(16) . ?
U5 O15 1.781(14) . ?
U5 O16 1.777(14) . ?
U5 O18 2.437(14) . ?
U6 U6 3.7513(15) 5_466 ?
U6 K3 4.027(5) 1_455 ?
U6 O2 2.438(14) 1_455 ?
U6 O7 2.359(14) 1_455 ?
U6 O14 2.236(16) . ?
U6 O17 1.798(14) . ?
U6 O18 1.883(15) . ?
U6 O19 2.309(13) 5_466 ?
U6 O19 2.270(13) . ?
Cd1 K2 3.557(9) 3_655 ?
Cd1 O1 2.335(19) . ?
Cd1 O1 2.335(18) 2_756 ?
Cd1 O5 2.581(17) 8_566 ?
Cd1 O5 2.581(17) 7_666 ?
Cd1 O20 2.374(16) 2_756 ?
Cd1 O20 2.374(17) . ?
K1 O4 2.984(16) 8_465 ?
K1 O4 2.984(16) 7_566 ?
K1 O9 2.919(15) . ?
K1 O9 2.919(15) 2 ?
K1 O13 2.809(15) 2 ?
K1 O13 2.809(15) . ?
K1 O15 2.947(15) 5_566 ?
K1 O15 2.947(15) 6_565 ?
K2 K3 3.701(14) 1_455 ?
K2 O8 3.102(15) 1_455 ?
K2 O8 3.102(15) 2_556 ?
K2 O17 2.726(15) 6_566 ?
K2 O17 2.726(15) 5_466 ?
K2 O18 2.685(16) . ?
K2 O18 2.685(16) 2_456 ?
K2 O20 2.714(16) 4_546 ?
K2 O20 2.714(16) 3_345 ?
K3 O4 2.852(17) 2_656 ?
K3 O4 2.852(17) . ?
K3 O7 2.931(15) 2_656 ?
K3 O7 2.931(15) . ?
K3 O8 3.238(16) . ?
K3 O8 3.238(16) 2_656 ?
K3 O18 2.888(16) 1_655 ?
K3 O18 2.888(16) 2_556 ?
O6 O6 0.92(5) 7_566 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
U1 U2 O4 K1 95.0(10) . . . 7_566 ?
U1 U2 O4 K3 -94.2(5) . . . . ?
U1 U2 O5 Cd1 20.2(13) . . . 7_666 ?
U2 U3 O9 K1 -65.4(8) 7_566 . . . ?
U2 U4 O13 K1 54.7(6) 7_566 . . . ?
U2 U6 O17 K2 -152.7(9) 1_455 . . 5_466 ?
U2 U6 O18 U5 -105.7(5) 1_455 . . . ?
U2 U6 O18 K2 113.1(7) 1_455 . . . ?
U2 U6 O18 K3 14.0(6) 1_455 . . 1_455 ?
U3 U4 O13 K1 -9.8(7) . . . . ?
U3 U5 O15 K1 -103.7(12) 2_556 . . 5_566 ?
U3 U6 O17 K2 -88.1(8) 1_455 . . 5_466 ?
U3 U6 O18 U5 -171.1(5) 1_455 . . . ?
U3 U6 O18 K2 47.7(7) 1_455 . . . ?
U3 U6 O18 K3 -51.4(5) 1_455 . . 1_455 ?
U4 U2 O4 K1 26.6(9) 7_566 . . 7_566 ?
U4 U2 O4 K3 -162.5(6) 7_566 . . . ?
U4 U2 O5 Cd1 88.3(13) 7_566 . . 7_666 ?
U4 U3 O9 K1 -8.3(9) . . . . ?
U4 U4 O13 K1 -78.5(7) 5_566 . . . ?
U4 U5 O15 K1 66.4(12) . . . 5_566 ?
U4 U5 O15 K1 -50.6(12) 2_556 . . 5_566 ?
U5 U3 O9 K1 -33.7(19) 2_556 . . . ?
U5 U4 O13 K1 -6.4(17) 2_556 . . . ?
U5 U4 O13 K1 164.7(3) . . . . ?
U5 U5 O15 K1 2.8(11) 2_556 . . 5_566 ?
U5 U6 O17 K2 103.4(8) . . . 5_466 ?
U5 U6 O18 K2 -141.2(11) . . . . ?
U5 U6 O18 K3 119.7(9) . . . 1_455 ?
U6 U2 O4 K1 163.8(9) 1_655 . . 7_566 ?
U6 U2 O4 K3 -25.4(6) 1_655 . . . ?
U6 U2 O5 Cd1 -48.7(12) 1_655 . . 7_666 ?
U6 U3 O9 K1 166.1(9) 1_655 . . . ?
U6 U5 O15 K1 138.7(12) . . . 5_566 ?
U6 U6 O17 K2 -19.1(8) 5_466 . . 5_466 ?
U6 U6 O18 U5 119.9(5) 5_466 . . . ?
U6 U6 O18 K2 -21.3(7) 5_466 . . . ?
U6 U6 O18 K3 -120.4(5) 5_466 . . 1_455 ?
K3 U2 O4 K1 -170.9(15) . . . 7_566 ?
K3 U2 O5 Cd1 -72.8(16) . . . 7_666 ?
K3 U3 O9 K1 -143.5(6) . . . . ?
K3 U6 O17 K2 -143.9(5) 1_455 . . 5_466 ?
K3 U6 O18 U5 -119.7(9) 1_455 . . . ?
K3 U6 O18 K2 99.1(9) 1_455 . . . ?
O2 U2 O4 K1 127.9(10) . . . 7_566 ?
O2 U2 O4 K3 -61.2(6) . . . . ?
O2 U2 O5 Cd1 -12.8(13) . . . 7_666 ?
O2 U6 O17 K2 169.7(9) 1_455 . . 5_466 ?
O2 U6 O18 U5 -68.6(6) 1_455 . . . ?
O2 U6 O18 K2 150.2(7) 1_455 . . . ?
O2 U6 O18 K3 51.1(6) 1_455 . . 1_455 ?
O3 U2 O4 K1 62.4(10) . . . 7_566 ?
O3 U2 O4 K3 -126.7(6) . . . . ?
O3 U2 O5 Cd1 52.7(13) . . . 7_666 ?
O3 U4 O13 K1 92.4(8) 7_566 . . . ?
O6 U2 O4 K1 -84.5(13) 7_566 . . 7_566 ?
O6 U2 O4 K1 -85.8(13) . . . 7_566 ?
O6 U2 O4 K3 85.1(10) . . . . ?
O6 U2 O4 K3 86.4(10) 7_566 . . . ?
O6 U2 O5 Cd1 -158.7(15) . . . 7_666 ?
O6 U2 O5 Cd1 -160.8(16) 7_566 . . 7_666 ?
O7 U2 O4 K1 -163.4(10) . . . 7_566 ?
O7 U2 O4 K3 7.4(6) . . . . ?
O7 U2 O5 Cd1 -81.4(14) . . . 7_666 ?
O7 U3 O9 K1 -156.0(10) . . . . ?
O7 U6 O17 K2 -123.2(8) 1_455 . . 5_466 ?
O7 U6 O18 U5 -136.3(6) 1_455 . . . ?
O7 U6 O18 K2 82.5(8) 1_455 . . . ?
O7 U6 O18 K3 -16.6(6) 1_455 . . 1_455 ?
O8 U5 O15 K1 -121.4(12) 2_556 . . 5_566 ?
O10 U3 O9 K1 28.7(10) . . . . ?
O10 U4 O13 K1 -113.8(8) 5_566 . . . ?
O10 U4 O13 K1 -44.2(8) . . . . ?
O11 U2 O4 K1 -5.4(10) 7_566 . . 7_566 ?
O11 U2 O4 K3 165.5(6) 7_566 . . . ?
O11 U2 O5 Cd1 120.5(13) 7_566 . . 7_666 ?
O11 U3 O9 K1 -44.4(10) . . . . ?
O11 U4 O13 K1 25.1(8) . . . . ?
O12 U5 O15 K1 36.3(12) . . . 5_566 ?
O12 U5 O15 K1 -32.0(12) 2_556 . . 5_566 ?
O14 U4 O13 K1 166.7(7) . . . . ?
O14 U5 O15 K1 101.7(12) . . . 5_566 ?
O14 U6 O17 K2 96.4(9) . . . 5_466 ?
O14 U6 O18 U5 5.0(5) . . . . ?
O14 U6 O18 K2 -136.2(8) . . . . ?
O14 U6 O18 K3 124.7(7) . . . 1_455 ?
O18 U5 O15 K1 167.6(12) . . . 5_566 ?
O19 U3 O9 K1 130.0(9) 5_566 . . . ?
O19 U6 O17 K2 16.2(9) . . . 5_466 ?
O19 U6 O17 K2 -53.7(9) 5_466 . . 5_466 ?
O19 U6 O18 U5 154.5(6) 5_466 . . . ?
O19 U6 O18 U5 84.5(6) . . . . ?
O19 U6 O18 K2 -56.7(8) . . . . ?
O19 U6 O18 K2 13.3(8) 5_466 . . . ?
O19 U6 O18 K3 -155.8(6) . . . 1_455 ?
O19 U6 O18 K3 -85.8(6) 5_466 . . 1_455 ?
